dynamic modeling of blownfilm...
Embed Size (px)
TRANSCRIPT

Dynamic Modeling of BlownFilm Extrusion
J. CARLPIRKLE, JR., andRICHARD D. BRAATZ
600 South Mathews Avenue, Box C3 University of lZlinois at UrbanaChampaign
Urbana, Rlinois 61 801
Past dynamic studies of blownfilm extrusion have been confined to the stability analysis of the linearized equations. The full set of nonlinear equations comprises a system of partial differential and algebraic equations with boundary conditions that vary from author to author. In this paper, the NumericalMethodofLines, which combines finitedifference methods with ordinary differential/algebraic equation inte grators, is used to solve the full system. Appropriate boundary conditions are selected to give physical results that compare well with experiment. An important boundary condition is the "minimum order reduction" condition on the gradient of the bub bletube radius with respect to distance above the extrusion die (the axial position). Transient startups and operational disturbances are examined. Calculations show the influence of oscillations in operating conditions such as heat transfer or inflation pressure on the bubbletube radius and film thickness. Steadystate results obtained by integrating the transient equations for a sufficiently long time are qualitatively in agreement with experiment, in contrast to past simulations of these equations.
INTRODUCTION
lown film extrusion is used to manufacture plas B tic bags and sheets of thin thermoplastic films (1). Although sign&cant effort has been made in the steadystate analysis of blown film extrusion, little has been attempted other than linearized stability analysis for the dynamic modeling of this process. Dy namic modeling enables the examination of strategies for process startup, for handling process upsets, and for process control.
Here the system of PDEs for the dynamic modeling of blown film extrusion is solved using Numerical MethodofLines (NMOL) (2). The dynamic and steady state solutions are presented for the PearsonPetrie model (3, 4), which has been a mainstay for modeling blown film extrusion of thin films. The NMOL method (spatial discretization of variables and approximation of derivatives by finite differences, followed by time in tegration to steadystate) avoids the instability of shooting methods used to solve steadystate equa tions directly. We show that the NMOL method yields steadystate results that are qualitatively different from the simulation results reported for the Pearson Petrie model by Liu et d (5). Furthermore, our results are in good qualitative agreement with the experimen tal results (6). This finding is important, because the steadystate simulation results obtained by Liu caused him to advocate an alternative model, the quasicylindrical model, to the thin shell model of Pearson and Petrie. This quasicylindrical model was used by subsequent researchers (7).
This paper describes the blown film extrusion pro cess, presents the dynamic equations for Pearson Petrie model, discusses some steadystate results (ob tained from the dynamic model at long times), and examines the dynamic response of the model to both startup and various process disturbances.
DESCRIPTION OF THE BLOWN FILM EXTRUSION PROCESS
Molten polymer is extruded through an annular die while air is fed through an inner concentric bubble tube (see Rg. 1 ) . This internal air causes the cylindri cal film to inflate, increasing the radius of the polymer bubble by stretching it, and decreasing the film thick ness. Simultaneously, the guide rolls above the die flatten the film and the nip rolls subject the film to tension in the axial (upward from the die) direction. External air supplied from a concentric outer ring cools the film. The resulting temperature reduction in creases the viscosity of the rising film and eventually induces crystaUization as the temperature drops be low the melting point of the polymer. The crystalliza tion, in turn, causes an additional increase in viscos ity, and the polymer solidifies.
The solidification zone is called the freeze zone or frost zone (1). Within this region, the rapidly increas ing viscous stiffness causes the bubble radius and the film thickness to stabilize, changing very little as the film heads upward toward the nip roils. The nip rolls and the bubble inflation create an elongating force on the polymer bubbletube. Also, the inflating air causes
398 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2

Dynamic Modeling of BlownFilm Extrusion
H +
Fig. 1 . Schematic of blown Jzh extrusion
a circumferential tension on the bubbletube. The re sulting biaxial stress can further induce crystalliza tion, an action termed flowinduced crystallization. Al though this effect has been included in a recent paper (7). it is neglected in most models of blown film extru sion (8, 9, 10).
Pearson and Petrie and others have developed steadystate models to describe the blown film extru sion process in the limit of very thin films (1 1, 12). In these models, variations of the physical variables across the thin film are neglected, leaving the vari ables as functions of axial position (height above the die) only. Generally, these models involve the continu ity equations, momentum equations in the axial and circumferential directions, and some type of constitu tive relation. In later applications, these were coupled with equations for energy and crystallization kinetics in order to follow the effect of temperature and crys tallization on the viscosity (5, 13).
PREVIOUS DYNAMIC MODELS
The timedependent equations for the thin film model of blawn film extrusion have been presented by various authors (8, 10, 14). The equations were lin earized in order to pedorm stability analysis, but so lutions for the original nonlinear equations were not presented. Owing to differences in numerical methods and constitutive relations, there is some disagreement in the results reported by these investigators.
Freeze Zone
Guide Rolls
AP
R # <
I Air
Yeow (14) presented the unsteadystate extension of the PearsonPetrie model for blownfilm extrusion. He derived the dynamic deformation rate tensor for the moving film and performed a stability analysis on the linearized version of the dynamic equations. Cain and Denn (8) followed up this work using a finite differ ence method and found qualitatively and quantatively Werent results. Yoon and Park (10) rederived the dy namic equations and performed another linearized stability analysis.
In this paper, we solve the dynamic continuity and momentum equations by the numerical method of lines (2). These equations are augmented with the dy namic energy balance equations and the constitutive relation used by Liu et aL (5), which allows reduction in viscosity by stressinduced deformation thinning as well as an increase in viscosity by temperature reduc tion and crystallization.
DYNAMIC PEARSONPETRIE MODEL
Like the steadystate PearsonPetrie model, the dy namic model of film motion neglects inertial terms, sur face tension, drag effects of the cooling air, and gravity. Dimensionless variables are used in the equations that follow. The dimensional and dimensionless variables are defined in Tables 1 and 2, respectively. The axial position variable 2 is bounded by 2 = 0 at the die and 2 = L at the upper boundary of the frost zone, which is called the frost line. The frost zone begins at the onset
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 399

J. Carl Pirkh, Jr., and Richard D. Braatz
Table 1. Symbols for Variables and Constants: Dimensional.
b CP c3 HO H HL kcrys L NZ R
VL VO Z
Exponent for denominator term of viscosity factor Specific heat of polymer Coefficient in crystallization rate expression Film thickness as it exits the die at Z = 0 Film thickness at axial position Z Film thickness at top boundary of freeze zone Crystallization rate coefficient Axial position corresponding to top boundary of freeze zone Number of grid points in discretization of axial coordinate Radius of film bubble tube at axial position Z Final radius of film bubble tube at top boundary of freeze zone Radius of film bubble tube as it exits the die at 2 = 0 Time Temperature of film bubble tube at position 2 Temperature of cooling air Equal to Tg  30 K, where Tg is the polymer glass transition temperature Melt temperature of polymer Temperature of film bubble tube as it exits die at 2 = 0 Activation energy for segmental jump rate in polymers Velocity of film at axial position Z Velocity of film at top boundary of freeze zone Velocity of film as it exits the die at 2 = 0 Axial position measured upward from position of die Adjustment coefficient for viscosity factor Adjustment coefficient for crystallization term in viscosity factor Adjustment coefficient for temperature dependence of viscositv factor Exponent for crystallization dependence of viscosity factor Local fraction of crystallinity Final crystallinity Heat of crystallization Inflation pressure, relative to ambient pressure Relaxation time Second invariant of the deformation rate tensor Polymer density Universal gas constant Viscosity of polymer Viscosity of polymer as it exits die
of crystallization and ends where further changes in bubbletube dimensions are imperceptible because of the extremely large viscosity. In simulations L is taken to be sufficiently large that the bubble tube is in this frozen state at 2 = L.
In the PearsonPetrie thin shell model, the dynamic continuity equation takes the dimensionless form (10):
(1)
where $ = dl + (ar/as)'. The dynamic momentum equation in the axial direction is:
r ah rhy ay rhav m a h + 87 llr3 a7 q2 as q~~ as
F, + B(r2  r 3 27
++
where ar y = , as (3)
F, is the dimensionless machine tension, B is the di mensionless inflation pressure defined in Table 2, and r, is the value of the dimensionless bubble radius r at s = L/R, and time 7. For the purpose of computing steadystate results and subsequent interpretation, the modified tension F = F,  Brf2 is used in this paper. The modified tension F is especially useful as a continuation parameter in getting around turning points when generating blowup ratio versus thickness reduction plots.
The dynamic momentum equation in the circumfer ential direction is:
The boundary conditions for the PearsonPetrie model have been the subject of some discussion. At the die, the three boundary conditions for bubble tube radius, film thickness, and film velocity are
r = l at s = O , (5)
400 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2

Dynamic Model ing of Blown& Extrusion
Table 2. Symbols for Variables and Constants: Dimensionless.
B F Modified tension Fln Dimensionless machine tension h r rL
V
VL Takeup ratio = VL/V, Y
r) e Dimensionless temperature = T/T, eair
Dimensionless pressure force = AP R,*/[2 po H, V,]
Dimensionless film thickness = HIH, Dimensionless film bubbletube radius = WR, Dimensionless film bubbletube radius at top boundary of freeze zone
Dimensionless film velocity = V/V,
Dimensionless derivative of radius with respect to axial position = ar/as
Dimensionless viscosity factor = p/k
Dimensionless temperature of air = T&T,
X Dimensionless crystallinity = WX,
s Dimensionless axial position = Z/ R,
V 7
Dimensionless frequency of oscillation, cycles per dimensionless time unit Dimensionless time = t V,/R,
JI Dimensionless curvature
h = l at s = O ,
u = l at s = O ,
respectively.
suggested boundary conditions are For the axial gradient of the bubbletube radius, the
y = y o at s = O (84 or
or
B 4J2 at s = L/Ro rl
(84
The first choice corresponds to the emergence of the molten polymer from the die at some preset angle to the vertical direction (e.g., yo = 0 for perfectly parallel flow). The difficulty with the fist boundary condition is the tendency for the melt leaving the die to expand or contract instantly. The second boundary condition is equivalent to cessation of the bubbletube expansion at the top boundary of the frost zone 2 = L. The prob lem with this boundary condition is the tendency for the gradient of the bubbletube radius to become ex ceedingly small anyway because of the stiffening of the polymer, and the imposition of Eq 8 b creates a non physical kink at s = L&. The last boundary condition (Eq 8c) results from setting @/as to zero in Eq 4. This type of boundary condition has been discussed and implemented by Schiesser (2) in the context of general convectiondiffusion equations, in which extensive lit erature has been written on the selection of outflow boundary conditions (15). We show later that Eq 8c is the preferred boundary condition at s = L/&.
The energy balance and crystallization equations are
 + +   B B , F , ( l  x ) = O ax ax a7 as
where
uh RO B , = P Cpf HOVO
Here, the heatloss term takes the form of Newtons law of convective cooling. Heat loss due to radiation is about 20% of that due to convection, so the effect of radiation has been lumped into the convection term by increasing the heat transfer coefficient U,. The function F, is the temperaturedependent factor for the rate of crystallization:
F, = 0 for e 2 8, (144
where the dimensionless constants B,,, %, Om, and 8, are
U* BFl = 
!Yl To
c3
T2, BF2 = 
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 401

J. Carl Pirkle, Jr., and Richard D. Braatz
402 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2
Tm
= To 0 = 
Like previous studies of blownfilm extrusion (an ex ception being Doufas and McHugh (7)), flowinduced crystallization is ignored.
The temperature and degree of crystallization are specified at the die
CONSTITUTIVE RELATION
A nonNewtonian constitutive relationship for de scribing the viscosity of the polymer during its extru sion, that takes deformation thinning into account, is (5)
where the base viscosity po is
and the dimensionless viscosity factor 11, which ac counts for temperature change and crystallization, is
Here, aI, az, PI , Pz. and b are measured or adjusted constants, and IId and A are the second invariant of the deformation rate tensor and the relaxation time, respectively. In terms of the dependent variables, the expression for nd is
Whenever A = 0, Eq 23 describes a Newtonian fluid. Equation 23 was elected for the calculations re
ported here as it was the constitutive relation used by Liu et d (5). This allows a direct comparison of re sults obtained with our numerical method and the in clusion of the exit boundary condition, Eq 8c, with those of Liu.
NUMERICAL METHOD OF SOLUTION
The above system of algebraic and partial differential equations is solved using the numerical method of lines (NMOL) (2). This involves discretizing the equations in the spatial variable s at a number of grid points N,. Spatial derivatives such as a v/a s are approximated as fivepoint finite differences in order to achieve 4thorder accuracy, thus eliminating the spatial variable as an in dependent variable. A variablegrid spacing technique
that allows a choice of such Spoint finite differences is coded in the subroutine DSS032 (16). The spatial discretization converts Eq 1 , 2, 4, 8c, 9, and 10 to a set of (5N, + 1) coupled ordinary differential equa tions containing time derivatives for the values of r, h, y, 0, and x at each grid point. Upon discretization, Eq 4 gives a set of N, algebraic equations (no time deriva tives). The boundary conditions (Eqs 5, 6, 7. 19, and 20) are included in the DAE system as algebraic equations.
The resulting system of or differential and al gebraic equations (DAEs) is solved using the double precision version of the solver DASSL (17, 18). All computations were performed in double precision For tran using a 900 M H z Athlon processorbased com puter. In coding the dynamic equations, the first grid point was selected at the beginning of the die ( Z = 0). Then the discretized equations were written for each grid point before moving on to the next. This resulted in a banded Jacobian that greatly speeded up the cal culations with DASSL.
The calculations started with 41 grid points, which were increased until the computed results were un changed within a minimum of four sigmficant figures of accuracy. The grid point allocation that met this criterion was 71 points uniformly distributed from s = 0 to 0.4, and 30 points uniformly distributed from s = 0.4 to 1.0. Spatial derivatives were approximated by using fivepoint biased upwind differences for ar/as, ah/as, av/as, aO/as, and ax/& and using fivepoint centered differences for ay/& (which is equal to a2r/as2).
The startup condition used in the calculations con sisted of extruding and attaching the bubble tube to the nip rolls under conditions of uniform (with respect to 2) bubbletube radius and film thickness. The two stress constants B and F, are then increased from zero to positive values by using the switching func tions:
B( 1  exp(  T"/T:))
where T~ is a switching time constant that can be set to be fast or slow, depending on the simulation. The switching function goes from zero to one as increases from zero.
The value of B is dependent on the pressure differ ence AP across the film, as shown in the definitions of Table 1. Whenever a given steadystate takeup ratio is desired, F, (or F) is adjusted until the takeup ve locity reaches the desired value. The adjustment of F, (or F) is accomplished by regula falsi interpolative root finding (19).
SIXULATIONS OF PEARSONPETRIE MODEL Table 3 contains the operating conditions for the
simulation and also gives the values for the physical parameters. The values of parameters associated with

Dynamic Modeling of BlownFitm Extrusion
Table 3. Values of Constants Used in Simulations.
4.68 s 0.68
85,000 K2 0.095 cm 2670 s 0.746 crn 331 K 118 K 414 K 463 K 50.27 W/rnzK 6284 kJ/krnol 0.366 cmls 0.96 Pas 13.5 4480 K 0.4 0.44 293.2 kJ/kg 919 kg/rn3 1 .o
2.43 kJ/kgK
the constitutive relation were obtained from the exper imental work of Liu et d (5, 6, 20, 21). They corre spond to a low density polyethylene (LDPE) provided by Dow Chemical Company. The inflation pressure AP ranged from 0 to 270 Pa. The takeup ratio vL. which is the film velocity at 2 = L divided by the film velocity at 2 = 0, varied from 2.988 to 5.200, and the temper ature To exiting the die varied from 443 to 467 K.
As most of the previous simulations for blownfilm extrusion were at steady state, the steadystate re sults of our model are first compared with the results of other investigators. Here the dynamic computations are carried out for a long enough period of time that the steady state was reached (in our case T = 5000 was used, which was more than sufficient). The mini mally reduced outflow boundary condition 8c was used as extensive computations showed that it yielded
the most physically meaningful results. As discussed below, the results for the other boundary conditions, 8a and 8b, contain nonphysical kinks in the solution near the entrance and exit boundaries, respectively, even when many grid points were assigned to those regions.
After discussing the steadystate results, dynamic calculations corresponding to boundary condition 8c are presented.
SteadyState Results of PearsonPetrie Model
Effect of Inttion Pressure
Flgure 2 shows the bubbletube radius correspond ing to various values of inflation pressure AP when the outflow boundary condition ( E q 8c) is used. The radius increases with 2 for inflation pressure AP = 250 and 270 Pa and decreases with 2 for AP = 0 and 150 Pa. The radius profiles flatten out for 2 > 10 cm because of the large increase in viscosity associated with decreasing temperature and increasing crystal linity. The blowup ratio ( h a l radius/initial radius) in creases with inflation pressure AP as expected. For an inflation pressure AP slightly above 270 Pa, the bub ble becomes unstable and the bubbletube radius ap proaches infinity, simulating a burst bubble.
Figure 3 gives the film thickness for the conditions corresponding to Flg. 2. The stretching force caused by increasing inflation pressure AP causes decreased film thickness H. At steady state, film velocity at each axial position 2 is given by mass continuity as V = VoHo&/HR, assuming constant density. During tran sition to steady state, the relationship among V, R, and H is more complicated.
Flgure 4 reports the blowup ratio (r at s = L / Q and thickness reduction (l/h) for the stable steadystate solutions computed for set values of B and F. For a fured inflation pressure B, there is only one steady state solution that intersects with the takeup ratio line (v = 2.988 at s = L/R,). This implies that the
I I I I I I I
Om2 0.0  0 5 10 15 20 25 30
Axial Position 2, cm
FYg. 2. Bubbletube radius p r o m s us. inJlation pressure AP: steadystate, To = 463 K, uL = 2.988.
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 403

J. Carl Pirkle, Jr., and Richard D. Braatz
0.10 0.09 0.08 0.07 0.06 0.05 0.04 0.03 0.02 0.01 I I I I I I 0.00 1 I I I I I 1
0 5 10 15 20 25 30
Axial Position Z, cm
Fig. 3 . Film thickness [email protected] us. infition pressure AP: steadystate, To = 463 K, v, = 2.988.
3.0
2.5
0 2.0
5 1.5
. Ic1
d
g = 1.0 0.5
0.0
p F=O. 148  0 Pa
0 1 2 3 4 5 6 7 8 9 1 0 1 1 1 2
Thickness Reduction Hg. 4. Blowup ratio us. thickness reduction for constant values of injhtwn pressure: steadgstate, To = 463 K.
blowup ratio increases monotonically with the inflation pressure. In generating the curves in FUJ. 4, the modi fied tension F was progressively reduced from the value indicated on the lower right of each curve to the value indicated on the upper part of each curve. The modi fied tension F was a good continuation parameter for getting around the turning points in the curves corre sponding to AP = 250 and 270 Pa.
The results shown in Figs. 2 and 4 do not exhibit the nonintuitive qualitative behavior reported by Liu and coworkers (5, 20, 21) when attempting to simu late the steadystate PearsonPetrie model. As the in flation pressure is increased, our results show an in crease in blowup ratio rather than the decrease reported by Liu and coworkers in their simulation
paper (5). Unlike their simulation results, our results are in agreement with their experimental findings (6). Liu and others (5, 22) used a boundary condition at the die exit (y = 0 at s = 0), a special case of Eq 8a (with yo = 0). which differs from the one we used, Eq 8c. This difference in boundary condition may be re sponsible for their contradictory simulation results.
For a given value of the inflation pressure AP, adding a small amount of viscoelasticity to the consti tutive relation has the effect of shifting the blowup ratio versus thickness reduction curves upward and to the right. This favors higher blowup ratios and thinner films. From the work of previous investigators (8, 22, 23), viscoelasticity is expected to increase sta bility by the strainhardening effect.
404 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2

Dynamic Modeling of BlownFilm Extrusion
Figures 5 and 6 show the temperature and crystal linity profiles for the various values of the inflation pressure AP. For inflation pressures of 250 Pa and 270 Pa, the flattening of the temperature for interme diate axial position Z is due to crystallization, which releases heat. As indicated in Eq 9, the rate of temper ature decrease with respect to axial position Z is smaller dimensionless film thickness h. As shown in Rg. 6, the lower temperatures result in more crystal lization for higher values of inflation pressure AP. This is expected, as E q 14 indicates that the rate of crystal lization becomes nonzero when the temperature drops below the melt temperature Om and increases as tem perature continues to drop.
The effect of crystallization on bubbletube stabiliza tion is profound. At X = 0.44, film viscosity, repre sented by Eq 23 and the parametric values in Table 3, is increased by seven orders of magnitude from that of the melt emerging from the die.
The axial gradient, y = aR/dZ, of the bubbletube radius R is plotted in Fig. 7 for various values of infla tion pressure AP. For inflation pressure AP = 250 and 270 Pa, the axial gradient y increases after the film leaves the die, and then declines rapidly to zero when reaching the frost zone at 2 > 8 cm. At inflation pres sure AP = 189.8 Pa, the radius profile remains per fectly flat for all values of 2 i.e., the axial gradient y = 0 uniformly. For inflation pressure AP = 0 and 150 Pa, the axial gradient y is negative as the film leaves the die, that is, the bubbletube contracts. As the axial position 2 increases, the axial gradient y ap proaches zero. Some investigators have solved the steadystate equations for blown film extrusion by
guessing the axial gradient y at the die exit (2 = 0) and using a shooting method to achieve some type of boundary condition at 2 = L (5, 22). Others have started by assuming that the axial gradient y = 0 at 2 = L, and using a shooting method to get the correct boundary conditions on the variables at Z = 0 (24,25, 26). In our case, and that of Cain and Denn (8). dis cretizing the axial position Z from 2 = 0 to 2 = L and using finite difference approximations to spatial deriv atives allows the direct satisfaction of any down stream boundary condition. As mentioned, the results reported here are for the downstream boundary con dition on the axial gradient y represented by E q 8c.
Effect of Machine Tension To examine the effect of machine tension on steady
state results, we found that the use of the modified tension F = F,  Brf2 was more revealing than using F,. For a die exit temperature of 463 K and conditions given in Table 3, the modified tension F was varied from 0 to a finite value to determine the range of infla tion pressures that yielded stable solutions. Corre sponding to each value of F, there is a lower and upper inflation pressure that allows physical solutions. Above the maximum inflation pressure, the radius grows un controllably, indicating a burst bubble. As shown in %. 8, the minimum inflation pressure is zero from F = 0 to F = 0.3450, but rises rapidly to equal the max imum inflation pressure at F = 0.4377. In the range between F = 0.3450 and F = 0.4377, as AP ap proaches the minimum inflation pressure from above, the bubble radius collapses to an infinitesimal quan tity, mimicking a vanishingly thin filament traveling
480 % Fm 460
!! 440 3 420 2i
400
380  360 ii
340
3
0 5 10 15 20 25 30
Axial Position Z, cm F'ig. 5. Film temperature projiles us. hfitionpressure AP: steadystate, To = 463 K, v, = 2.988.
POLYMER ENGlNEERlNG AND SCIENCE, FEBRUARY 2OU3, Vof. 43, No. 2 405

J. Carl Pirkle, Jr., and Richard D. Braakz
0.50 0.45 0.40 0.35
c 0.30 r
0.25
8 0.15 (II
5 0.20
0.1 0 0.05 0.00
0 5 10 15 20 25 30
Axial Position Z, cm Flg. 6. Crystallinity proms us. i n t n pressure AP: steadystate, To = 463 K, v, = 2.988.
at ever increasing speed. For F = 0 to 0.4377, there is no stable solution for inflation pressures either above the maximum or below the minimum. Above F = 0.4377, there is no stable solution for any inflation pressure.
In the negative range of the modified tension, F = 0 to 0.13. the maximum inflation pressure continues
to decline, while the minimum inflation pressure rises above zero. Actually, a solution does exist below the minimum inflation pressure, but it corresponds to negative values of F,, a nonoperable condition. For F < 0.13, F, is always negative.
Use of the modified tension F in Fig. 8 instead of the tension F, gave more revealing plots of the allowable
0.20
0.1 5 * * f 0.10
0.05 (3  =% x 0.00 4
0.05
0.1 0 0 5 10 15 20 25 30
Axial Position Z, cm Flg. 7. Awial gradient proms us. inJlatbn pressure AP: steadystate, To = 463 K, u, = 2.988.
406 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2

Dynamic Modeling of BlownFilm ExmLswn
250 Q L
g 200 a
2 150 u) u)
P S 0
c c
._ z 1 
00
50
0
I r I t +Upper limit I t I I Lower limit1 I
I
0.2 0.1 0 0.1 0.2 0.3 0.4 0.5
Modified Tension F PTg. 8. Upper and lower i n t t i o n pressure bounds as afunction of n w d i i tension F.
ranges of inflation pressure AP (or B) as F varied mo notonically while F, sometimes exhibited nonmonoto nic behavior.
Effect of Die Ekit Temperature
To examine the effect of die exit temperature To upon the process variables, the inflation pressure was set to AP = 250 Pa and the takeup ratio to vL = 2.988. All other conditions being equal, the bubble radius is expected to grow larger as the die exit temperature To is increased due to the reduction in viscosity. The ra dial profiles corresponding to die exit temperature To = 443, 463, and 468 K are given in Q. 9. The radius profiles increase with the die exit temperature To, which, unlike the computed results of Liu (20, 21), is physically reasonable.
Other Eflects: Spatiall9 Variable lnfrcltion Pressure and Heat lrtansfer Cmmients
In order to make a oneonone comparison with the calculations of Liu et al. (20, 21), the calculations just presented corresponded to spatially uniform inflation pressure and heat transfer coefficients. For complete ness, however, we examined some other effects on the calculated steadystate results.
Fitst, the heat transfer coefficient and the inflation pressure were varied spatially according to the calcu lated aerodynamic profiles of the external cooling air by Akaike et al. (9). These investigators used the kE method discussed by Abe et al. (27). Their calcula tions showed that the exterior surface pressure on the bubbletube was negative near the die, followed by a rise to a positive value and then a decline to nearly zero. As a consequence, the inflation pressure AP cor responding to an inside bubbletube pressure of 270
Pa gauge, had the profile shown in Q. 10. In con trast, the heat transfer coefficient uh calculated by Akaike et al. increased from a low value of approxi mately 10 W/(m2K) at the die to a higher value of ap proximately 190 W/(m2K) in the frost zone (about 7 10 cm) and then declined to a small value down stream of the frost zone (see Fig. 1 I ) . Sidiripoulos and Vlachapoulos (28) calculated similar behavior and at tributed it to a combination of Coanda and Venturi ef fects.
Thus, the emerging melt near s = 0 would be sub jected to a lower cooling rate and a higher inflation pressure than occurs in the case of constant uh and AP. This combination of occurrences should threaten the stability of the bubbletube at the entrance zone (near o = 0) as it is subjected to greater stress while the viscosity of the melt is at its lowest value. In the case of the deformation thinning model in Eq 23. the bubbletube burst at an extrusion temperature at To = 463 K. A lower extrusion temperature, To = 457.46 K, was required to keep the bubbletube stable while achieving a similar blowup ratio. For a nondeforma tionthinning model, e.g., one corresponding to A = 0, the bubbletube is less vulnerable to instability in the entrance zone near h. = 0, but the extrusion tempera ture To must be higher, about 488 K.
Another spatial profile for U,, based on the work of Kanai and White (29). was mentioned by Liu (20, 21). In this expression, uh was held constant at uh,o from Z = 0 to Z = Z,,, and then allowed to drop off as U,,0/Z2.5. Our calculations showed that this dropoff had very little effect on the results as long as 2 was a few centimeters past the beginning of the frost zone. At this point, the film viscosity was several orders of mag nitude higher than at Z = 0, and the geometric vari ables R and H were stabilized. As mentioned earlier.
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 407

J. Carl Pirkle, Jr., and Richard D. Braatz
0.20
1.80
i i I
1.60
1.40
E 0 1.20 a 1.00 .I 2 0.80 m
0.60
0.40 I I
0.00 ' I I I I I 1 0 5 10 15 20 25 30
Axial Position Z, cm Fig. 9. Effect of die exit temperature To upon bubble radius profles.
,
0 5 10 15 20 25 30
Z, cm Fig. 10. Qpical prom of [email protected] pressure resdtingfrom aerodynamics of external cooling air: reference (91.
crystallization played a large role in the increase in viscosity. and a lack of cIystallization would result in less film stability for the Kanai and White model.
Comparison of Boundary Conditions for the Axial Gradient y
There is some debate over the proper boundary con dition for the axial gradient y of the bubble radius r.
Here is a demonstration of why the oufflow boundary condition 8c, which is called the "minimum order re duction" condition by Schiesser (30), was used. For the case of inflation pressure AP = 270 Pa and take up ratio vL = 2.988, Fig. 12 compares steadystate profiles of the axial gradient y for boundary conditions 8a and 8c. The value of the axial gradient at the die, yo, corresponding to boundary condition 8a is taken
408 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vof. 43, No. 2

Dynamic Modeling of BlownFilm Extrusion
Y C;r E <
z 5
m
Flg. 1 1 .
t
0 5 10 15 20 25 30
Z, cm ll~pical p r o m of heat transfer [email protected] r e s w f r o r n aerodynamics of extemal cooling air: refmence (9).
to be zero. The boundary condition 8a yields a non physical kink in the value of the axial gradient at the die exit, as it suddenly rises to attain nearly the same values as the plot for Eq 8c. If the correct value of the axial gradient y = yo at the die exit was known, then the boundary condition 8a could be used without a kink occurring in the entrance zone of the solution. But, of course, the value for yo is not known in ad vance.
In Flg. 13, profiles for the bubbletube radius R ob tained using the different boundary conditions 8b and 8c are compared. There is a severe nonphysical wiggle at 2 = L when boundary condition 8 b is used. Such nonphysical wiggles due to this form of exit boundary condition are described in some detail by Schiesser (30). Refining the grid points did not eliminate this wiggle. For this reason, the outflow boundary condi tion 8c was used.
0.050 0.045 0.040 0.035 0.030 0.025 0.020 0.01 5 0.01 0 0.005 0.000 c r I I I
0 2 4 6 8 10
Axial Position Z, cm Fig. 12. Comparison of awial gradient p r o m s obtainedfrom boundary conditions 8a and 8c.
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 409

J. Carl Pirkle, Jr., and Richard D. Braatz
E K
5
0
v) 3
a K
1.2
1 .o
0.8
0.6
I i i
I I I I I
10 15 25
Axial Position Z, cm Ffg. 13. Comparison of bubbletube radius profis obtainedfrom boundary conditions 8b and 8c.
Dynamic Behavior of PearsonPetrie Modal
Several investigators have studied the dynamics of the PearsonPetrie model by linearizing the nonlinear equations and computing the eigenvalues (8, 10, 14, 31). Here the transient nonlinear equations are solved to observe the evolution of process variables from startup to steady state. Specifically, we examine the effect that the shifting time has on the transition of process variables from one steady state to another. Also, the sensitivity of process variables to oscillations in the operating conditions is observed. In particular, the effects of variations of heat transfer coefficients, the inflation pressure AP, and the machine tension F upon the process operations are investigated.
kansient ShiJ Between Steady States
Of practical interest is how smoothly the blown film extrusion process can be shifted from one steady state to another. For the simulations here, the die exit tem perature To = 463 K, the takeup ratio vL = 2.988, and the rest of the conditions are given in Table 3. The ini tial dimensionless inflation pressure B = 0.0654080 (this corresponds to AP = 125 Pa) and the modified tension F = 0.28376298. After the initial steady state is reached, the inflation pressure and machine ten sion are shifted to new values of B = 0.1308200 (this corresponds to AP = 250 Pa) and F = 0.31031428, re spectively. In the simulation, the mathematical func tion used for the shift was
F,, = Fold + (Fne,  Fold)[ 1  expf 72/7:h13)1 (28) Because disturbances are rapidly propagated by the momentum balance (Eq 2) in the axial direction, the takeup ratio does not remain at 2.988 during this transition. Rather, the takeup ratio will experience a transitory departure in its steadystate value. The na ture of this departure depends on the value of T ~ , the shifting time, as indicated in Flg. 14. The longer the shifting time, the less the excursion of the takeup ratio v,, and the smoother the transition. At a shifting time of 30. which is roughly the travel time of the film from 2 = 0 to 2 = L, the spike in vL is greatly reduced. For below 20, the velocity profile overshoots and then sometimes undershoots its steadystate value. The major concern from the perspective of process opera tion is that this gyration in film velocity will cause wrinkling of the sheet unless the transition between steady states is made sufficiently gradual.
Flgwes 1520 show how the dimensions and prop erties of the polymer bubble develop with respect to time using a shifting time T~~ = 30. All of the profiles in Fgs. 1520 develop smoothly with time, nearly reaching steady state in about 300 seconds (about 10 times L/V& Figure 15 shows that bubbletube radius at low axial positions responds more quickly than at the highest axial position (2 = L). This is to be ex pected, since changes in the polymer film take time to
41 0 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2

Dynamic Modeling of BlownFilm Extrusion
m. 14. Takeup ratio V, after a shift in rnod~w tension and [email protected] tion pressure.
U 3
Y & 3.1 s
3
l  'shift = 'shift =
. . . .
= 15 = 30
  'shift '  ' 'shift
0
propagate to the higher axial positions. A similar ef fect is seen in the film thickness (see Fig. 16) and temperature profiles (see Rg. 18). Also, the crystdin ity profile climbs to its new steadystate value, reach ing the maximum allowed value ( X = 0.44) at 2 = L (see Fig. 19). This dynamic effect is related to the con stant value of crystallinity for 2 = L achieved for a range of inflation pressure (see Rg. 6). Likewise, the axial gradient y of the bubbletube radius progres sively increases to its new steadystate profile (see Fig. 20). Similar behavior was observed for other values of the inflation pressure, die exit temperature, and take up ratio.
Oscillations in Operating Conditions Heat transfer from film to cooling air. In many ex
perimental and smaller commercial blown film ex truders, externally and internally flowing air streams
2.9 *
Q. 15. Bubbletube radius pro files after shift to new inJlatwn pressure AP and modw tension F (rSmfi = 30).
10 20 30 40 Time z, dimensionless
cool the polymer film as it leaves the die. Roper cool ing is important to get an acceptable viscosity profie and to obtain proper crystallization. The rate of cool ing affects the dimensions (bubbletube radius and film thickness) and strength of the bubble tube. The coefficient for film to air heat transfer U, depends on the physical properties of the air as well as the pat tern of flow in the boundary layer next to the film. In the calculations that follow, the inflation pressure AP = 265 Pa, the timeaveraged takeup ratio v, = 2.988, and the die a i t temperature To = 463 K. The other conditions and physical properties are given in Table 3.
The heat transfer coefficient was assumed to be a sinusoid with frequency v and amplitude of either 2% or 4% of the steady value (the bubble was unstable for constant values of the heat transfer coefficient above 4% of the nominal value). The maximum positive and negative deviations of the final bubbletube radius
1.1 E 1.0 0 u 0.9 v) 0.8 3 5 0.7 2 0.6 I
0.4 0 5 10 15 20 25 30
Axial Position Z, cm
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 41 1

J. Carl Pirkle, Jr., and Richard D. Braatz
0.01 0.00
0.1 0 0.09
1
1
5 0.08 f 0.07 $ 0.06 a C 0.05 Y 0
* 0.04 c 0.03 0.02
1.2
1 .o
0.8
8 2 0.6
0.2 0 5 10 15 20 25 30
Axial Position Z, cm Q. 17. Nrn velocity projlks after shiff to new infition pressure AP and modified tenswn F IT,,, = 30).
412 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2

Dynamic Modeling of BlownFilm ESmusion
470
450
Y .. 430 2 3
2 410 Q) Q
fii 390 I
370
350
CI
1 I I I
0 5 10 15 20 25 30
Axial Position 2, cm FYg. 18. Film temperature p r o m s a m shi. to new injhtion pressure AP and machine tension F ( T ~ ~ = 30).
0.5
0.4
0.3
0.2
0.1
0.0
0 5 10 15 20 25 30 Axial Position 2, cm
FYg. 19. Crystallinity [email protected] a m ship to new injlation pressure LW and d i @ e d tension F [ T ~ ~ ~ = 30).
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 41 3

J. Carl Pirkle, Jr., and Richard D. Braatz
, 0.05 I I
I a .I
2
0.04
0.03 .I Q) 0.02
0.01
0.00
0.01
0.02
D
0.03 I I i I I 1 0 5 10 15 20 25 30
Axial Position Z, cm FYg. 20. Axial gradient of bubbletube radius proms [email protected] shift to n e ~ ~ injlation pressure AP and modpd tension F ( T ~ , , ~ = 30).
(that is, the radius r, at the top of the freeze zone) as a function of frequency of oscillation are shown in Q. 21. The frequency of variation of r, follows the fre quency in the oscillation of the heat transfer coeffi cient Uh extremely closely and is practically equal to Y. The positive and negative deviations, r,  rL,ss, are not symmetric about zero. This lack of symmetry can be attributed to the nonlinearity of the system with re spect to the temperature effect on the viscosity. As ex pected for a physical system, the maximum deviation declines rapidly at higher frequencies.
The mean variation rL,m (upper value minus lower value of r,  rL,ss divided by two) is plotted versus fre quency u in FQ. 22 for amplitudes of oscillation in heat transfer coefficient uh of 2% and 4%. The maxi mum mean variation in rLSm (for low values of uh) is sensitive to variation in the heat transfer coefficient uh. At low frequencies, changes of 2% and 4% in the heat transfer coefficient uh correspond to changes in the bubbletube radius r, of 6.4% and 17.4%. respec tively. The maximum mean variation is more than two ordersofmagnitude smaller for frequencies higher than 0.32.
There is a kink in the plots around the frequency 0.2. The kink persisted when the calculations were re peated for increasing number of grid points, suggest ing that the kink is a real characteristic of the dy namic relationship between heat transfer coefficient variations and the bubbletube radius. This kink sug gests a partial separation of time scales in the dy namic behavior of the process. These time scales are not easily attributed to single groups of governing equations because of their coupling.
Inflation air Dressure. Here is a determination of the effect of oscillations of the inflation pressure on the operation of blown film extrusion. The base inflation pressure is 265 Pa, the machine tension F is held at 0.3 1 1, and the amplitude of oscillation is taken be ei ther 1.2% or 2.4%. For constant values of machine tension above 2.4%, the bubble was unstable and burst. For a 2.4% variation of inflation pressure about the inflation pressure AP = 265 Pa, Flg. 23 shows the maximum positive and negative deviations in the final bubbletube radius rL as a function of frequency Y. The deviations are not symmetrical about zero (and hence the dynamic behavior is significantly nonlin ear), and the deviations do not decrease monotonically with frequency. At the frequency u = 0.12. the devia tions reach a local minimum in magnitude, then climb to a local maximum at u = 0.15 before resuming a de crease toward zero. At low frequencies, small changes in the inflation pressure AP cause large changes in the bubbletube radius r,, with 1.2% and 2.4% varia tions in AP resulting in 7.8% and 25.2?40 maximum variation, respectively, in rv
The mean deviation in the bubbletube radius r, (upper value minus lower value of r,  rL,ss divided by two) is plotted as a function of frequency u in Q. 24 for 1% and 2% amplitude in variations of inflation pressure AP about 265 Pa. Here the local minimum and maximum are more evident in the region Y = 0.12 to 0.15. The maximum mean variation is more than two ordersofmagnitude smaller for frequencies higher than 0.1 than for low frequencies.
Machine tension. Here is an investigation of the ef fect of oscillating machine tension on the behavior of
414 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2

Dynamic Modering ofBlownFilm Extrusion
0.5
0.3
0.2
0.1
0.0
0.1
0.2 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7
Frequency v
I I I
m. 21. M & m deviation of&& bubble radius as afunction of thefrequency of oscillation of the heat transfer coemient U,.
the blown film extrusion process. The base value of the modified tension F is taken as 0.3 1 1, and the am plitude of oscillation is taken as 11.5% around this value. The maximum deviations of the bubbletube radius r, as a function of the frequency of oscillation are shown in Fig. 25. Unlike the cases involving heat
transfer or inflation pressure, the upper and lower values of the maximum deviation are relatively sym metrical with respect to zero, which occurs for linear relationships between variables. The maximum devia tions in the bubbletube radius are similar in magni tude for oscillations in inflation pressure and machine
6i 0 J
  0 T I
1
1.5
2
2.5
3 I I I I i 2 1.5 1 0.5 0
Log,o Frequency FXg. 22. Mean mDximLun amplitude of deviawn in t h e m bubble radius rL resullingfrom 2% and 4% variation in the heat transfer coefficient U,.
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 41 5

J. Carl Pirkle, Jr., and Richard D. Braatz
0.50
0.40
0.30
0.20
0.10
0.00
0.1 0
0.20 0.00 0.05 0.10
Frequency v
0.15 0.20
Q. 23. M a x i m u m deviation of thefinal bubble radius r, as afunction of thefrequency of oscillation of in_flation pressure AP.
0
0.5
1
1.5
2
2.5
3
3.5 2.5 2 1.5
Log,o Frequency
1 0.5
Q. 24. M e a n mQyimum amplitude of deviation offinal bubble radius r, resulwfrom oscillation of the injlatbnpressure AP.
416 POLYMER ENGlNEERlNG AND SCIENCE, FEBRUARY 2003, Vof. 43, No. 2

Dynamic Modeling of BlownFilm Exhuswn
0.40 I I <
0.30  Positive deviation  0.20
 Negative deviation
1 0.20
0.30 I I I I I I 0 0.1 0.2 0.3 0.4 0.5 0.6
Frequency v lQg. 25. Maximum deuiation of theJnal bubble radius rL as afunction of thefrequency of oscillation of the [email protected] tension F (1 1.5% amplitude].
tension (compare Figs. 23 and 25), although the rela tive maximum change in machine tension was much greater than the maximum change in inflation pres sure (2%). This indicates that the bubbletube radius is much more sensitive to oscillations in the inflation pressure than oscillations in machine tension.
In Fig. 26, the mean maximum deviation in r, is plotted as a function of frequency u for the 11.5% am plitude in oscillation of the modified tension F. The rolloff of the amplitude is much more gradual as a function of frequency than for the heat transfer co efficient and inflation pressure, indicating that high
.E . s g .o = E
0.5
1
1.5
 2.s f I I I I . 2 1.5 1 0.5 0
Log,, Frequency
Fg. 26. M e a n maximum amplitude of deviation of$ml bubble radius rL resulting from oscillation of the [email protected]@d tension F (1 1.5% amplitudel.
POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2 41 7

J. Carl Pirkle, Jr., and R i c h d D. Braatz
frequency oscillations in the machine tension have a stronger relative effect. This result agrees with physi cal intuition, since high frequency oscillations in ma chine tension rather directly affect the bubble geome try, whereas the effect of high frequency oscillations in heat transfer coefficient and inflation pressure receive more damping by the thermal and physical inertia of the polymer film. The maximum mean variation is one orderofmagnitude smaller for a frequency of 0.27 than for low frequencies.
CONCLUSIONS When the NMOL approach is used to solve the two
point boundary value problem that comprises the PearsonPetrie thin film blown film extrusion model, the results are in good qualitative agreement with ex periment. The bubbletube radius is seen to increase with inflation pressure under a wide range of condi tions. This suggests that the "counterintuitive" simu lation results of Liu and coworkers (5, 20, 21) and Ashok and Campbell (22) resulted from application of an incorrect boundary condition (Eq 8a) or numerical inaccuracies exacerbated by not knowing the true val ue of the axial gradient y at the die exit. The boundary conditions and numerical method used here avoid such problems.
When the blown film process is started up, under goes a deliberate change, or suffers an upset, the dy namic model can be easily solved to predict the out come. The dynamic model readily reveals the effect of oscillations in operating conditions such as heat trans fer, inflation pressure, or machine tension on film bub bletube dynamics. The dynamic model can be used to quantify the extent of nonlinearity between relevant process variables, or to design process control systems.
ACI(N0WLEDGME"IS The authors thank Mitsuko Fujiwara for help in
manuscript preparation, and the National Center for Supercomputing Applications and Procter and Gam ble for support.
REFERENCES 1. S. Middleman, FundnmentQl Studies of Polymer Process
ing, McGrawHill, New York (1977). 2. W. E. Schiesser, The Numerical Method of Lines Integra
tion of Partial Dtferential Equations, Academic Press, San Diego (1991).
3. J. R. A. Pearson and C. J. S. Petrie, J . Fluid Mech, 40, l(1970).
4. J. R. A. Pearson and C. J. S . Petrie, J. Ffuid Mech, 42,
5. C.C. Liu, D. C. Bogue, and J. E. Spruiell. Intern. Polyrn.
6. C.C. Liu, D. C. Bogue, and J. E. Spruiell, Intern Polyrn
7. A. K. Doufas and A. J. McHugh, J. of Rheology, 46,
8. J. J. Cain and M. M. Denn, Polyrn Eng. Sci., 28. 1527
9. 0. Akaike, T. Tsuiji. and Y. Nagano, Intern. Polym Pro
10. K.S. Yoon and C.W. Park, Intern. Polyn Process., 14.
11. C. J. S. Petrie, AlChEJ., 21, 275 (1975). 12. K.S. Yoon and C.W. Park, Polyrn Eng. Sci, 32, 1771
13. S. M. Alaie and T. C. Papanastasiou, Intern. Polym Pro
14. Y. L. Yeow, J. Fluid Mech, 75, 577 (1976). 15. R. A. Novy, H. T. Davis, and L. E . Scriven, Chem. Eng.
Sci, 46, 57 (1991). 16. C. A. Silebi and W. E. Schiesser. Dynamic Modeling of
Transport Process Systems, p. 409. Academic Press, San Diego (1992).
17. L. R. Petzold, "A description of DASSL: a differential/al gebraic system solver," In R.S. Stepleman, ed., Scientii
18. T. Maly and L. R. Petzold, Appl. Numer. Math., 20, 57
609 (1970).
Process., 10, 230 (1995).
Process., 10, 226 (1995).
1085 (2001).
(1988).
cess., 14, 168 (1999).
342 (1999).
( 1992).
cess., 8, 51 (1993).
C O ~ U ~ , pp. 6568, IMACS, NorthHolland (1983).
19.
20.
21.
22.
23.
24.
25.
26.
(1996). F. Scheid, Numerical Analysis, p. 311, McGrawHill, New York (19681. C.C. Liu, Studies of Mathematical Modelling and Experi mental OnLine Measurement Techniques for the Tub Film Blowing Process, M.S. thesis, Dept. of Materials Science and Engineering, University of Tennessee, Knox ville (1991). C.C. Liu, OnLine Experimental Study and Theoretical Modelling of Mular Film Blowing, Ph.D. thesis, Dept. of Materials Science and Engineering, University of Ten nessee, Knoxville (1994). B. K. Ashok and G . A. Campbell, Intern Polyrn Process., 7 , 240 (1992). K . 6 . Yoon and C. W. Park, J . NonNewtonian Fluid Mech, 89,97 (2000). X.L. Luo and R. I. Tanner, Polyrn Eng. Sci, as, 620 (1985). J. R. A. Pearson and C. J. S. Petrie, Plast. Polym, 38. 85 (1970). T. Kanai and J. L. White, J. Polgrn Eng., 6, 3277 (1975).
27. K. Abe, T. Kondoh, and Y. Nagano, IGnt J. Heat & M a s s
28. V. Sidiropoulos and J. Vlachopoulos, Polyrn Eng. Sci.
29. T. Kanai and J. L. White, Polyn Eng. Sci, 24, 1185
30. W. E. Schiesser, AppL Nwner. Math., 20, 171 (1996). 31. H. Andrianarahinjaka and P. Micheau, Comptes Rendus
de L'Acadernie des Sciences Series IIBMechanique, Physique. Chimie, Astronomic, 322,363 (1996).
Trmfm, 388, 1467 (1995).
40, 1611 (2000).
(1984).
41 8 POLYMER ENGINEERING AND SCIENCE, FEBRUARY 2003, Vol. 43, No. 2